Abstract
Despite their seemingly random appearances in the real space, quasirandom nanophotonic structures exhibit distinct structural correlations and have been widely utilized for effective photon management. However, current design approaches mainly rely on the deterministic representations consisting twodimensional (2D) discretized patterns in the real space. They fail to capture the inherent nondeterministic characteristic of the quasirandom structures and inevitably result in a large design dimensionality. Here, we report a new design approach that employs the onedimensional (1D) spectral density function (SDF) as the unique representation of nondeterministic quasirandom structures in the Fourier space with greatly reduced design dimensionality. One 1D SDF representation can be used to generate infinite sets of real space structures in 2D with equally optimized performance, which was further validated experimentally using lighttrapping structures in a thin film absorber as a model system. The optimized nondeterministic quasirandom nanostructures improve the broadband absorption by 225% over the unpatterned cell.
Introduction
Unlike the conventional photonic crystals with periodic structures, quasirandom nanostructures comprise seemingly random material distributions governed by underlying structural correlations. Their quasirandom geometries lead to rich Fourier spectrums that are highly desirable for wideangle and broadband light control^{1, 2}. Such class of nanostructures was discovered in the feathers and scales of multiple lineages of birds and insets for producing noniridescent colors to fulfill biological functions, such as camouflage, intimidation and communication^{2,3,4,5,6,7,8,9,10,11,12,13}. Taking the inspiration from nature, manmade quasirandom nanostructures have also been developed for various optical applications including energy harvesting^{14,15,16,17,18}, lightemitting diodes^{19}, random lasing^{20, 21}, structural coloration^{22, 23}, plasmonic quasicrystals^{24}, transmission and reflection controlling^{25,26,27,28}.
Apart from their unique characteristics, the design of the quasirandom nanophotonic structures fundamentally differs from the one for their periodic counterparts, mainly due to their inherent nondeterministic nature. To better illustrate this, let us consider several representative cases of the quasirandom structures featuring both channeltype and disktype morphologies (Fig. 1). Two quasirandom nanostructures with channeltype morphology are shown in Figure 1a and b, which can be obtained via the spinodal decomposition process^{9, 29}. On the other hand, Figure 1c shows a disktype quasirandom structure that can be obtained from nucleation process^{30}. Interestingly, despite their drastically different real space appearances, the twodimensional (2D) Fourier transformations of these structures exhibit very similar ringshaped patterns as shown in Figure 1d,e. The similarity in the Fourier space not only reveals the underlying structural correlation in common but further suggests their similar characteristics in light scattering or diffraction modes.
However, this observed onetomultiple mapping from the Fourier space characterization to the real space geometries has been unfortunately overlooked. The current design approaches mainly rely on the deterministic representation of the quasirandom structures in real space^{31, 32}. The geometry is first represented using discretized pixels and the material occupations at each pixel are then optimized for the targeting performance. While this real space design approach has seen successes in optimizing periodic photonic structures^{31, 33}, it fails to capture the inherent nondeterministic characteristic of the quasirandom structures and inevitably results in a large design dimensionality^{31}. Furthermore, in view of the observed onetomultiple mapping, there are infinite real space patterns that can all satisfy the same design objective by sharing the same type of Fourier spectrum. However, the design based on the real space representation can only provide one specific solution among the infinite choices of quasirandom patterns and thus, lose the genericity of the obtained optimal solution.
On the contrary, the naturally occurring quasirandom nanostructures feature nondeterministic material distributions and are created via extremely scalable and low cost phase separation processes^{9}. We recognize that the distribution of the Fourier components in reciprocal space provides a unique structural representation of the nondeterministic quasi random systems and captures the characteristic of lightmatter interaction at the same time. As shown in Figure 1d–f, the concentration of the Fourier components over the narrow range of spatial frequencies in these Fourier spectrums indicates the welldefined correlation length, which has been demonstrated to largely determine the light scattering characteristics of the nanostructures. Therefore, designing the quasirandom structure directly in Fourier space provides a more attractive solution that can simultaneously capture both characteristics of structural correlation in the real space and the light scattering in the reciprocal space.
Results
In this work, we use the spectral density function (SDF), a onedimensional (1D) function as the normalized radial average of the square magnitude of the Fourier spectrum, to provide a unique representation of the structure in the reciprocal space. For a twodimensional quasirandom structure Z(r) with binary value at each location r to represent the material occupation, the SDF f(k) can be obtained based on the Fourier transformation of Z(r) as Eq. 1:
where A _{ k } and ϕ _{ k } represent the magnitude and phase information at each k of the Fourier transform, and k is a frequency vector having the same dimension as Z(r). When the quasirandom structure Z(r) is isotropic, the vector k can be reduced to a scalar k. Thus, f(k) becomes a onedimensional function f(k) that satisfies \(f(k)=\,f({\bf{k}}=k)\), and C in Eq. (1) is a normalizing constant that ensures the integral of f(k) over the considered spatial frequency domain as 1.
The underlying mathematical connection between the real space structural correlation function, i.e. twopoint correlation function, and the Fourier spectrum has been well established based on the WinnerKhinchin theorem^{34}. Thus, the SDF essentially characterizes the structural correlation information in the reciprocal space. Meanwhile, by describing the distribution of Fourier components over spatial frequency, this characterization method has been utilized for predicting the reflectance spectra of nanostructure in analyzing biological structure color systems^{6, 35}. Therefore, the SDF unifies the underlying structural correlation and characterizes the lightmatter interaction. By recognizing the axial symmetry in their Fourier spectra, we propose the onedimensional SDF as a unique representation of the nondeterministic quasirandom nanophotonic systems in two or three dimensions. Therefore, in contrast to the deterministic pixelated realspace structure representation, infinite numbers of the real space quasirandom structures can be generated using statistical reconstruction methods^{36, 37} based on a given SDF structural representation.
To demonstrate the capability of using SDF for representing and reconstructing quasirandom nanophotonic structures, different forms of SDF are tested as shown in Figure 2. Based on a SDF following a Gaussian distribution shown in Figure 2a, a channeltype and a disktype quasirandom structure are reconstructed as shown in Figure 2c and d, respectively. Here, we develop two noniterative reconstruction methods based on SDFs, i.e. the Gaussian random field (GRF) modeling for the channeltype structures and the random packing algorithm (RPA) for the disktypes (see Method Section). Corresponding to the identical SDF, the two structures in Figure 2c and d possess dispersed Fourier spectra as shown in the insets of Figure 2c and d, which implies that their structural correlation spreads over a range of spatial distance. For comparison, a twostep shaped SDF and the two reconstructed structures with different real space morphology types are displayed in Figure 2b,e and f, respectively. The reconstructed structures in Figure 2e and f present a hierarchical geometry with features at two length scales corresponding to the two distinct frequency bands in Fourier space. This interesting feature implies these structures possess structural correlations in two separated spatial ranges. Figure 2g–j display another 4 different SDFs, i.e. the decreasinglinear function in Figure 2g, the increasinglinear function in Figure 2h, the tripledelta function in Figure 2i, and the truncated Gaussian distribution in Figure 2j. Figure 2k–n show the quasirandom structures reconstructed from the SDFs in Figure 2g–j. The distributions of the Fourier components of these structures as shown by the insets of Figure 2k–n correspond to their SDFs. As demonstrated in Figure 2, most SDFs as the nondeterministic representations of the quasirandom structures can be mathematically formulated based on less than 5 governing parameters, which significantly reduces the design dimensionality of such complex systems. Furthermore, since our reconstruction methods are applicable to arbitrary forms of SDF, we can generate the structures mimicking the selfassembled structure from certain bottomup process by utilizing the corresponding SDF derived in literature^{38}.
Utilizing SDF for structural representation and reconstruction, we developed a new simulationbased design approach for optimizing quasirandom nanophotonic structures by exploiting the design representation in the Fourier space, as outlined in Figure 3a. Instead of following the conventional approach that tailors the real space structure in 2D, our approach optimizes the 1D SDF f(k) in the Fourier space as the design representation of the structure with reduced dimensionality. Once the SDF design representation is initialized, the 2D realspace quasirandom structures are reconstructed by GRF or RPA methods. The optical performance of these reconstructed structures are then evaluated using the rigorous couple wave analysis (RCWA) or the Finitedifferent timedomain (FDTD) method. Based on the evaluation, the SDF parameters are updated using optimization algorithm. Finally, the optimized structures in real space are reconstructed based on the optimized SDF which is obtained from the iterative optimization loop.
Our method is mainly focused on the design of the quasirandom nanophotonic structures that exhibit unique polarizationindependent optical characteristic. This is often originated from the lack of the longrange translational ordering in the quasirandom structures, which results in the observed rotational symmetry in the twodimensional (2D) spectrum in the Kspace. Thus, in our method, the onedimensional (1D) spectral density function (SDF) is used as the unique design representation of the 2D quasirandom photonic structures, which is in clearly contrast to the other Kspace based approaches that mainly rely on the use of full 2D Fourier spectrum as the design representations^{25, 26, 39}. While the use of 1D SDF as the design representation offers the immediate benefit with significant dimensionality reduction of the design space, more importantly, it further enables the design of nondeterministic quasirandom nanophotonic structures, i.e. the structures of different realspace geometries featuring equivalent Fourier spectrum characteristics with rotational symmetry.
A lighttrapping structure in a silicon absorber is employed as a representative example to demonstrate this approach, as shown in Figure 3b. In this simplified model system, the top layer with the quasirandom structure is the lighttrapping layer of thickness t_{1}, which is directly patterned on the amorphous silicon (aSi) based absorbing layer with total thickness of t. The bottom silver layer prevents the light escaping on the back side. The lighttrapping structure is optimized for maximizing light absorption by balancing the competing processes of light reflection and scattering. The design objective is formulated in Equation 2:
where Z denotes the quasirandom lighttrapping structure depending on f(k) as the SDF, ρ as the material filling ratio and t _{1} as the patterning depth, A is the total light absorption to be maximized at targeting wavelength λ.
Our method does not impose any limitation on the formulation of the SDF and thus, designer has the freedom to formulate the SDF according to desired physics optical properties as the design objectives. For the demonstration of this capability, we choose the stepshaped SDF exhibiting bandpass characteristics in the kspace. The corresponding passband is defined within the range from k _{a} to k _{b}, which is shown in the inset of Fig. 3c. The unit of k _{a} and k _{b} is nm^{−1}. Since the material refractive index also significantly influences the absorption in lighttrapping process, the material filling ratio ρ of the quasirandom nanostructure is simultaneously designed. The thickness of the quasirandom nanostructured layer t _{1} is another design variable considered in this work. Comparing with the real space approach that involves thousands or millions of design variables due to the design space discretization, this Fourier space design approach with only four design variables, i.e. (k _{a}, k _{b}, ρ, and t _{1}), significantly reduces the design dimensionality, yet still directly captures the key factors that influence the performance.
In this work, the rigorous coupled wave analysis (RCWA)^{40, 41} is adopted to evaluate the light absorption coefficients of the reconstructed structures. RCWA is a Fourierdomainbased algorithm that can solve the scattering problems for both periodic and aperiodic structures. The length of the unit cell for RCWA calculation is set as 2000 nm. We studied the light absorbing characteristic of the superstructures formed by spatially tiling of 1) identical unit cells or 2) different unit cell patterns but originated from the same SDF. Theoretically, they are expected to exhibit the same light absorption. While different algorithms can be adopted for design updating, here we use the genetic algorithm (GA)^{33, 42, 43}. Mimicking natural evolution with the underlying idea of survivalofthefittest, GA is a stochastic, global search algorithm involving the iterative operation of selection, recombination, and mutation on a population of designs^{42, 43}. This simulationbased design loop iterates to search for the optimized design of quasirandom nanophotonic structures in Fourier space. Based on the optimized SDF and other variables, infinite sets of equally optimized structures in realspace can be generated via statistical reconstructions, using methods such as the GRF method or the RPA method.
Figure 3c–j display the optimization process and results of using our Fourier space design approach for a single wavelength λ = 650 nm. In this case, the thickness of the quasirandom lighttrapping structure is set as 100 nm and the total thickness of aSi layer t is set as 600 nm. Therefore, three design variables are considered in this single wavelength optimization case, i.e. k _{a} and k _{b} for the stepshape SDF and ρ for the material filling ratio. The optimization history is shown in Figure 3c, in which each dot represents the corresponding absorption coefficient for a given set of design variables (k _{a}, k _{b}, and ρ). Starting from the randomly generated initial designs with the absorption coefficient around 0.4, the optimization converges to the solution (k _{a}* = 0.0018 nm^{−1}, k _{b}* = 0.0030 nm^{−1}, and ρ* = 78%) with the absorption coefficient larger than 0.85. Statistical representation using SDF enables infinite numbers of optimized quasirandom structures to be generated in real space. Six 2 μmby2 μm designs were reconstructed based on the optimal solution denoted by the red triangles in Figure 3c, with the channeltype structures in Figure 3d–f generated using GRF method, and the disktype structures in Figure 3g–i generated using RPA method, respectively. Despite the different realspace morphologies, all designs possess similar ringshaped Fourier spectra and achieve the equal optimum performance. For further validation, shown in Figure 3j, 50 real space patterns were generated from the optimized design and evaluated to have an average absorption of 0.88 with less than 4% variation due to the discrete meshing in numerical calculation, thereby achieving a 225% enhancement of the absorption in the unpatterned cell.
Lastly, we conducted a broadband optimization of the quasirandom lighttrapping structures over the visible solar spectrum using our SDFbased design approach. In this case, the total thickness of the aSi layer t is set as 650 nm, and the thickness of the quasirandom structure t _{1} is considered as another design variable to demonstrate the strength of our approach. Four design variables (k _{a}, k _{b}, ρ and t _{1}) are optimized for the maximal light absorption over the solar spectrum from 400 nm to 800 nm. There are 81 wavelengths considered over the whole wavelength spectrum, and the objective is to maximize the aggregated absorption normalized by the singlepath absorption at each wavelength. The optimization converges to the solution (k _{a}* = 0.0012 nm^{−1}, k _{b}* = 0.0036 nm^{−1}, ρ* = 51%, t _{1}* = 150 nm), which leads to a donutshape Fourier spectrum as shown in Figure 4a,d,g. This optimized Fourier spectrum overlaps with the area defined by two dashed circles, which denote the range of kvectors for coupling the incident light to the quasiguided modes in the silicon film^{14, 31}. Three distinct lighttrapping designs in real space are realized from the identical optimized SDF. In Figure 4b, the first lighttrapping design is generated by repeating one single optimized unit cell, as denoted by the dashed window. A second design with channeltype morphology (Fig. 4e) and a third design with disktype morphology (Fig. 4h) also are generated by heterogeneous assembly among 25 different unit cells. It is observed here that the quasirandom structures shown in Figure 4e and h possess the rich, continuous Fourier spectra in Figure 4d and g, whereas the periodic structure with quasirandom unit cell in Figure 4b leads to discrete diffraction order in the Fourier spectrum shown in Figure 4a. The gradient of the color bar in Figure 4a has been adjusted to better visualize the discrete points in the Fourier spectrum.
Two reference structures with the same thickness of silicon material are compared with the optimized structures for the lighttrapping performance, including unpatterned cells with and without a 70 nm silicon dioxide antireflection coating (ARC). The simulated absorption spectra of the three optimized quasirandom structures and two reference cells are plotted in Figure 4j. The unpatterned cell shows overall low absorption except several high peaks due to the FabryPerot resonances occurred between the airsilicon interface and the bottom reflector. By adding the antireflection coating (ARC), the absorption in high absorbing region of aSi (400 nm–550 nm) is greatly enhanced, while the FabryPerot absorption peaks are suppressed due to the reduced reflection at the airsilicon interface. Furthermore, the cells with the three optimized quasirandom structures from the same SDF exhibit very similar broadband absorption characteristics over the entire spectrum, which is due to the combination of antireflection effect and more efficient light scattering. The enhancement in the strong absorbing region of aSi (400 nm–550 nm) is caused by the reduced refractive index mismatch between the air and the aSi, which is comparable with the ARC control case. The enhancement in weak absorbing region (550 nm–800 nm) is mainly due to the enhanced light scattering via the design optimization in the Kspace. The coupling to the socalled quasiguided mode results in the enhanced absorption of the incident light. The presence of efficient light scattering also effectively suppress the formation of the FabryPerot resonance. All three lighttrapping structures with drastically different realspace patterns enhanced the absorption by more than threefold in the weak absorbing region compared with the two references, achieving an average absorption coefficient of 0.74 over the broad spectrum from 400 nm to 800 nm. All three lighttrapping structures with drastically different realspace patterns enhanced the absorption by more than threefold in the weak absorbing region compared with the two references, achieving an average absorption coefficient of 0.74 over the broad spectrum from 400 nm to 800 nm. The difference between the absorption spectrums of the channeltype structure in Figure 4e and the disktype structure in Figure 4i is observed. This difference is likely due to the different structure reconstruction methods adopted for the two types of structures. The RPA based reconstruction that requires all the inclusion to have a disk shape has more geometrical constraints than GRF that can generate arbitrary geometries at small scale. Thus, from the same designated SDF, GRF can generate structures more accurately than RPA, resulting in the observed difference between the two absorption spectrums. However, the averaged absorbing performance of these two optimized structures over the targeting broadband is very similar.
The three optimized quasirandom structures were also fabricated on an aSi substrate and characterized experimentally (see Method Section), as shown in Figure 4c,f and i, respectively. Exhibiting a broadband enhancement, especially over the weak absorption region from 600 nm to 800 nm, the measured spectra of the optimized cells in Figure 4k agreed well with the simulation results. It should be noted that the spectroscopic details found in Figure 4j are caused by the interference of multiple scatterings from the pixelated fine features of the quasirandom pattern in Figure 4b,e,f. In contrast, those fine features such as sharp corners and small dots are diminished from the fabricated samples shown in Figure 4c,f,i, which result in much smoother experimentally measured curve. The quasirandom structure improved the absorption of this aSi absorber by 230% compared with unpatterned cell without ARC and 147% compared with unpatterned cell with ARC. In this work, the topdown method is employed to fabricate the quasirandom lighttrapping structure for conceptual validation. For other bottomup nanomanufacturing processes^{15, 28}, this design approach provides the design freedom to downselect the optimized structures that are compatible with the fabrication platforms. The manufacturing conditions can be further incorporated into the structure design by deriving the formulation of the SDF considering the governing physics of the corresponding bottomup processes^{29, 38}.
Discussion
In conclusion, we developed a new design approach by adopting the representation in the Fourier space to design the nondeterministic quasirandom nanophotonic structures. The nondeterministic structures in 2D were represented using 1D SDF. This representation in Fourier space not only captures the structural correlation and other key factors that collectively govern the light scattering characteristics of the quasirandom nanophotonic systems, but also significantly reduces the design dimensionality compared with the real space design approaches. We have demonstrated the versatility of the noniterative method to reconstruct the real space structures with different morphology types based on arbitrary forms of SDF. The Gaussian random field modeling is primarily used to reconstruct quasirandom patterns with “tortuous channellike” morphology, which can be observed in the processes such as the phase separation by Spinodal decomposition in the polymer blends. In contrast, the random packing algorithm is better suited to reconstruct quasirandom pattern exhibiting particlelike morphology. Thus, RPA can find more applications that relate to nucleation or nanoparticle assembly processes. Following an inverse design strategy, this SDF based approach enables the full exploitation of the potential of quasirandom nanophotonics for highperformance optical devices. It provides the design freedom to downselect the optimized structures that are compatible with the fabrication platforms. The manufacturing conditions can be further incorporated into the structure design by deriving the formulation of the SDF based on the governing physics of bottomup processes. Readily applicable to various nanophotonic applications, including lasing control, light coupler for LEDs, and structural coloration, this approach can be further extended to solve functional material design problems beyond the optical regime.
Method
Disktype quasirandom nanophotonic structure statistical reconstruction
For the disktype quasirandom nanophotonic structure shown in Figure 1c, we adopted the randomspherepacking method to generate the realspace pattern from the given spectral density function. As a statistical reconstruction method, this process achieves the nonoverlapping random packing of disks in 2D realspace or spheres in 3D realspace. Many efforts have been made toward the packing algorithm to achieve different geometric characteristics^{44,45,46}. In our work, we developed a new algorithm that packs the disks in 2D space or spheres in 3D space based on its SDF.
Using 2D disk packing as an example, the typical SDF of an equalsize random close disk packing structure in Figure 1c resembles dense hexagonal packings and has apparent periodicity. As a result, its Fourier spectrum its components concentrated on a single ring, i.e. a certain spatial frequency. Through our empirical studies, it is discovered that the radius of the ring in Figure 1f can be estimated based on the radius of disks packed in the structure: k = L/1.69∙r, where L is the side length of the structure and r is the radius of disks. More complex SDF profiles can be achieved by packing disks with different sizes. It was discovered from our empirical studies that the intensity of SDF f (k) at a certain frequency k _{ i } is proportional to the total area of the corresponding disk of radius r _{ i }, where k _{ i } and r _{ i } satisfy the relationship:
where N _{ i } is the number of disks of radius r _{ i }. In addition, when the total areas of disks for each size r _{ i } are equal, the corresponding f (k _{ i }) are equal. Based on these relationships, the appropriate disk sizes and number of disks can be estimated according to the magnitude of the spectral density over different frequencies and the target material filling ratio. The effectiveness of this packing algorithm is verified by structures with a variety of SDFs in Figure 2.
Channeltype quasirandom nanophotonic structure statistical reconstruction
To reconstruct the realspace structures with channeltype morphology as shown in Figure 1d for given spectral density functions and material filling ratio, Gaussian random field (GRF) modeling is adopted in this work. A standard GRF, denoted as Y(r), is a random field with all points jointly following a standard Gaussian distribution. A standard GRF over a ndimensional space is characterized by the fieldfield correlation function g(r _{1}, r _{2}) in Equation (4). Defined as the statistical correlation between two points, g(r _{1}, r _{2}) describes the fluctuation characteristic of the Gaussian random field. In Equation (4), J are Bessel functions of the first kind, f(k) is the spectral density function of a random variable k. Therefore, a GRF Y(r) is constructed for a given spectral density function f(k) following this relationship. Once the GRF is generated, as shown by Equation (5), the realspace, twophase, quasirandom structure Z(r) can be obtained by levelcutting the GRF Y(r) at α, which is determined by the material filling ratio.
Among the Gaussian random fields, a natural type that has been used to describe the morphology of a thermodynamic system in a phaseseparation process is the GaussMarkov fields. For this type of Gaussian random fields over the 3D space, the Landau free energy is local and a polynomial in (k ^{2})^{38}. The SDF describing such system is found in literature^{38} as shown in Equation (6), governed by three parameters, k _{0}, b, and t, with C as the normalization parameter. It has been discussed in the literature^{38} that the length scale of the structural feature in the corresponding channeltype quasirandom system is determined by (E[ k ^{2} ])^{1/2} = (b ^{2} + 2bk _{ 0 }cost)^{1/2} and the minimum feature is determined by the value of k as f(k) → 0. It is noted that the curve approaches to a δfunction with the peak at k = b when t → π/2. Other SDF formulations for different thermodynamic systems can be found in literature to describe the morphological characteristic of resultant quasirandom structures.
RCWA absorption evaluation and GA based optimization
In this work, the rigorous coupled wave analysis (RCWA) method is adopted to calculate the light absorption of the realspace quasirandom structures reconstructed from the SDF design representation. RCWA is one of the most commonly used techniques to solve the scattering problem in Fourier space. The length of the unit cell is determined to be 2000 nm in this work. SDF provides a statistical characterization of the structure and different realspace structures (isotropic) reconstructed from the same SDF are statistically equivalent in reciprocal space. The characteristics of the reciprocal space of the structure mostly determine their performance for photon management^{31}. Therefore, the lighttrapping performance of a quasirandom structure assembled from multiple statistically equivalent unit cells with different realspace geometries is theoretically as same as that of a structure as a periodic arrangement of a same unit cell. In this case, the RCWA calculation while assuming a periodicity boundary condition for either type of the structures returns the correct absorption values, which is validated in Figure 4j and k.
Based on the calculated absorption values, Genetic Algorithm (GA) is used to search the optimal design. The design variables are coded using the binary notation that are regarded as the chromosomes in GA. A population of the chromosomes went through the iterative operation of selection, recombination, and mutation, and converge to the optimal broadband, light trapping structure. Although GAs with different strategies of selection, recombination, and mutation have been developed, the strategy of selfadaptive mutation is used in this work^{47}. Here, the designs mutate by adding a random parameter with normally distribution to each design variable. The mutation strength (i.e., standard deviation of the normal distribution) was selfadaptive and varied during the optimization process. The strength increases as the optimization converges. We can observe this selfadaptive control of the mutation in the history plot of main text (Fig. 4a) where larger fluctuations occur at the late stage of the optimization (converged regime, after 186^{th} evaluation) than in the beginning stage (linear regime, before 130^{th} evaluation). In this work, the selfadaptive GA search is performed using the commercial optimization software iSight from Dassault Systemes.
Experimental section
The lighttrapping structure in thinfilm silicon absorber is adopted as the testbed for the SDF based design strategy to optimize quasirandom nanophotonic structures. Fabrication of the amorphous silicon (aSi) absorber begins with a 200 nm aluminum film deposited on a silicon wafer by an AJA electron beam evaporator. Next, on top of the aluminum reflector, the 600 nm aSi film was deposited by inductively coupled plasma chemical vapor deposition (ICPCVD, Oxford Plasmalab 100). In the aSi with ARC layer, the 70 nm silicon dioxide film was deposited by plasmaenhanced chemical vapor deposition (PECVD, STS LpX CVD). The thicknesses and optical properties of both aSi and silicon dioxide were characterized by ellipsometer (J. A. Woollam M2000U). The three quasirandom structures in Figure 4 were fabricated by focused ion beam (FEI Helios Nanolab SEM/FIB) milling (30 kV, 28 pA) on the aSi film with a patterned area of 60 μm by 60 μm. The reflection spectrum for each sample was measured by a grating spectrometer (Andor SR303i) with wavelength resolution of 0.6 nm combined with a Leica DMI 3000 M microscope. A tungsten lamp was used as a light source covering the spectral range from 400 nm to 800 nm. The reflection coefficient is then calculated by the using the experimentally measured reflection spectrum from an aluminum mirror as the reference. With 500 nm aluminum underneath the aSi, light transmitted through the sample is negligible. Thus, the absorption spectrum is obtained by subtracting the reflection coefficient from unity.
References
 1.
Wiersma, D. S. Disordered photonics. Nat Photonics 7, 188–196 (2013).
 2.
Shi, L. et al. Amorphous Photonic Crystals with Only ShortRange Order. Adv Mater 25, 5314–5320 (2013).
 3.
Vukusic, P. & Sambles, J. R. Photonic structures in biology. Nature 424, 852–855 (2003).
 4.
Parker, A. R. & Townley, H. E. Biomimetics of photonic nanostructures. Nat Nanotechnol 2, 347–353 (2007).
 5.
Kinoshita, S. i. Structural colors in the realm of nature (World Scientific, 2008).
 6.
Prum, R. O., Torres, R. H., Williamson, S. & Dyck, J. Coherent light scattering by blue feather barbs. Nature 396, 28–29 (1998).
 7.
Vukusic, P., Hallam, B. & Noyes, J. Brilliant whiteness in ultrathin beetle scales. Science 315, 348–348 (2007).
 8.
Yin, H. W. et al. Amorphous diamondstructured photonic crystal in the feather barbs of the scarlet macaw. P Natl Acad Sci USA 109, 10798 (2012).
 9.
Dufresne, E. R. et al. Selfassembly of amorphous biophotonic nanostructures by phase separation. Soft Matter 5, 1792–1795 (2009).
 10.
Dong, B. Q. et al. Structural coloration and photonic pseudogap in natural random closepacking photonic structures. Opt Express 18, 14430–14438 (2010).
 11.
Noh, H. et al. How Noniridescent Colors Are Generated by Quasiordered Structures of Bird Feathers. Adv Mater 22, 2871–2880 (2010).
 12.
Burresi, M. et al. Brightwhite beetle scales optimise multiple scattering of light. Scientific reports 4, 6075 (2014).
 13.
Siddique, R. H., Gomard, G. & Holscher, H. The role of random nanostructures for the omnidirectional antireflection properties of the glasswing butterfly. Nat Commun 6, 6909 (2015).
 14.
Vynck, K., Burresi, M., Riboli, F. & Wiersma, D. S. Photon management in twodimensional disordered media. Nature Materials 11, 1017–1022 (2012).
 15.
Kim, J. B. et al. Wrinkles and deep folds as photonic structures in photovoltaics. Nat Photonics 6, 327–332 (2012).
 16.
Smith, A. J., Wang, C., Guo, D. N., Sun, C. & Huang, J. X. Repurposing Bluray movie discs as quasirandom nanoimprinting templates for photon management. Nat Commun 5, 5517 (2014).
 17.
Aeschlimann, M. et al. Perfect absorption in nanotextured thin films via Andersonlocalized photon modes. Nat Photon 9, 663–668 (2015).
 18.
Schuster, C. S. et al. Plasmonic and diffractive nanostructures for light trappingan experimental comparison. Optica 2, 194–200 (2015).
 19.
Koo, W. H. et al. Light extraction from organic lightemitting diodes enhanced by spontaneously formed buckles. Nat Photonics 4, 222–226 (2010).
 20.
Noh, H. et al. Control of Lasing in Biomimetic Structures with ShortRange Order. Phys Rev Lett 106, 183901 (2011).
 21.
Liu, J. et al. Random nanolasing in the Anderson localized regime. Nat Nanotechnol 9, 285–289 (2014).
 22.
Forster, J. D. et al. Biomimetic Isotropic Nanostructures for Structural Coloration. Adv Mater 22, 2939–2944 (2010).
 23.
Zhang, Y. F. et al. Using Cuttlefish Ink as an Additive to Produce Noniridescent Structural Colors of High Color Visibility. Adv Mater 27, 4719–4724 (2015).
 24.
Achanta, V. G. Plasmonic quasicrystals. Prog Quant Electron 39, 1–23 (2015).
 25.
Kasture, S. et al. Plasmonic quasicrystals with broadband transmission enhancement. Scientific Reports 4 (2014).
 26.
Matsui, T., Agrawal, A., Nahata, A. & Vardeny, Z. V. Transmission resonances through aperiodic arrays of subwavelength apertures. Nature 446, 517–521 (2007).
 27.
Agrawal, A., Matsui, T., Vardeny, Z. V. & Nahata, A. Terahertz transmission properties of quasiperiodic and aperiodic aperture arrays. J Opt Soc Am B 24, 2545–2555 (2007).
 28.
Walheim, S., Schaffer, E., Mlynek, J. & Steiner, U. Nanophaseseparated polymer films as highperformance antireflection coatings. Science 283, 520–522 (1999).
 29.
Cahn, J. W. Phase Separation by Spinodal Decomposition in Isotropic Systems. J Chem Phys 42, 93& (1965).
 30.
Liu, W. & Gao, X. Reducing HAuCl(4) by the C(60) dianion: C(60)directed selfassembly of gold nanoparticles into novel fullerene bound gold nanoassemblies. Nanotechnology 19, 405609 (2008).
 31.
Martins, E. R. et al. Deterministic quasirandom nanostructures for photon control. Nat Commun 4, 2665 (2013).
 32.
van Lare, M. C. & Polman, A. Optimized Scattering Power Spectral Density of Photovoltaic LightTrapping Patterns. Acs Photonics 2, 822–831 (2015).
 33.
Wang, C., Yu, S. C., Chen, W. & Sun, C. Highly Efficient LightTrapping Structure Design Inspired By Natural Evolution. Scientific reports 3, 1025 (2013).
 34.
Champeney, D. C. A handbook of Fourier theorems (Cambridge University Press, 1987).
 35.
Prum, R. O., Dufresne, E. R., Quinn, T. & Waters, K. Development of colourproducing betakeratin nanostructures in avian feather barbs. J R Soc Interface 6, S253–S265 (2009).
 36.
Yeong, C. L. Y. & Torquato, S. Reconstructing random media. Phys Rev E 57, 495–506 (1998).
 37.
Torquato, S. Statistical description of microstructures. Annu Rev Mater Res 32, 77–111 (2002).
 38.
Teubner, M. Level Surfaces of Gaussian RandomFields and Microemulsions. Europhys Lett 14, 403–408 (1991).
 39.
Martins, E. R. et al. Deterministic quasirandom nanostructures for photon control. Nat Commun 4 (2013).
 40.
Li, L. F. New formulation of the Fourier modal method for crossed surfacerelief gratings. J Opt Soc Am A 14, 2758–2767 (1997).
 41.
Moharam, M. G., Pommet, D. A., Grann, E. B. & Gaylord, T. K. Stable Implementation of the Rigorous CoupledWave Analysis for SurfaceRelief Gratings  Enhanced Transmittance Matrix Approach. J Opt Soc Am A 12, 1077–1086 (1995).
 42.
Goldberg, D. E. Genetic Algorithms in Search, Optimization, and Machine Learning (AddisonWesley Professional, 1989).
 43.
Eiben, A. E. & Smith, J. From evolutionary computation to the evolution of things. Nature 521, 476–482 (2015).
 44.
Lubachevsky, B. D. & Stillinger, F. H. GeometricProperties of Random Disk Packings. J Stat Phys 60, 561–583 (1990).
 45.
Donev, A. et al. Improving the density of jammed disordered packings using ellipsoids. Science 303, 990–993 (2004).
 46.
Skoge, M., Donev, A., Stillinger, F. H. & Torquato, S. Packing hyperspheres in highdimensional Euclidean spaces. Phys Rev E 74, 041127 (2006).
 47.
Deb, K. & Beyer, H. G. Selfadaptive genetic algorithms with simulated binary crossover. Evol Comput 9, 197–221 (2001).
Acknowledgements
This work is supported by National Science Foundation under grants CMMI1130640 and EEC1530734. We thank Dr. David Czaplewski at Argonne National Lab in assisting with aSi deposition. The use of the Center for Nanoscale Materials, an Office of Science user facility, was supported by the U. S. Department of Energy, Office of Science, Office of Basic Energy Sciences, under Contract No. DEAC026CH11357. This work also made use of the EPIC facility and KeckII facility (NUANCE CenterNorthwestern University), which has received support from the MRSEC program (NSF DMR1121262) at the Materials Research Center; the Nanoscale Science and Engineering Center (NSF EEC–0647560) at the International Institute for Nanotechnology; and the State of Illinois, through the International Institute for Nanotechnology. S.Y. also thanks the International Institute for Nanotechnology for the Ryan Fellowship award.
Author information
Affiliations
Contributions
W.C. and C.S. initiated and supervised the project. S.Y. conceived the design framework and conducted the optimization with Y.Z. and J.Z., C.W., B.D. and X.C. conducted the sample fabrication and characterization. All authors discussed the results and contributed to the manuscript.
Corresponding authors
Ethics declarations
Competing Interests
The authors declare that they have no competing interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Yu, S., Wang, C., Zhang, Y. et al. Design of NonDeterministic Quasirandom Nanophotonic Structures Using Fourier Space Representations. Sci Rep 7, 3752 (2017). https://doi.org/10.1038/s4159801704013z
Received:
Accepted:
Published:
Further reading

Dewetting behavior of Ge layers on SiO2 under annealing
Scientific Reports (2020)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.